Abstract
Monolayer groupIII monochalcogenides (MX, M = Ga, In; X = S, Se, Te), an emerging category of twodimensional (2D) semiconductors, hold great promise for electronics, optoelectronics and catalysts. By firstprinciples calculations, we show that the phonon dispersion and Raman spectra, as well as the electronic and topological properties of monolayer MX can be tuned by oxygen functionalization. Chemisorption of oxygen atoms on one side or both sides of the MX sheet narrows or even closes the band gap, enlarges work function, and significantly reduces the carrier effective mass. More excitingly, InS, InSe, and InTe monolayers with doubleside oxygen functionalization are 2D topological insulators with sizeable bulk gap up to 0.21 eV. Their lowenergy bands near the Fermi level are dominated by the p_{ x } and p_{ y } orbitals of atoms, allowing band engineering via inplane strains. Our studies provide viable strategy for realizing quantum spin Hall effect in monolayer groupIII monochalcogenides at room temperature, and utilizing these novel 2D materials for highspeed and dissipationless transport devices.
Introduction
GroupIII monochalcogenides (MX, M = Ga, In; X = S, Se, Te) are layered semiconductors that have been extensively studied for decades due to their peculiar properties, such as high carrier mobility, sombreroshape valence band edges, rare ptype electronic behaviors, etc.^{1,2} It is not until recently that their few or monolayer sheets (GaS, GaSe, and InSe) are realized in experiment,^{3,4,5} constituting a new family member of twodimensional (2D) materials. Monolayer MX has a hexagonal lattice composed of two planes of metal atoms sandwiched between two planes of chalcogen atoms. These 2D sheets have band gap of 2.20–3.98 eV;^{6} the gap and electronic transport properties are layer dependent, rendering these materials promising candidates for electronic and optoelectronic devices.^{7,8,9} Recently, field effect transistors based on monolayer InSe were fabricated with ultrahigh carrier mobility above 10^{3} cm^{2} V^{−1} s^{−1} and large on/off ratio of 10^{8}.^{8,9} Photodetectors made of GaS, GaSe, GaTe, or InSe nanosheets exhibit high photoresponsivity and fast response time for a broad spectral range.^{3,4,10,11} Besides, these novel 2D compounds were demonstrated to be potential piezoelectric and thermoelectric materials,^{12,13} photocatalysts and electrocatalysts.^{6,14}
On the other hand, chemical functionalization of 2D materials is an effective strategy to tailor the material properties and trigger exotic phenomena. Oxidation and hydrogenation of graphene and silicene are widely exploited in experiment for band gap engineering.^{15,16} Other 2D honeycomb lattices modified by H, O, and halogen atoms are theoretically proposed, showing tunable and diverse electronic and topological properties. For instance, oxidation of monolayer blue phosphorus induces quantum phase transitions and novel emergent fermions,^{17} while hydrogenation and fluorination can create σcharacter Dirac cones.^{18} Quantum spin Hall (QSH) effects were predicted for the functionalized group IV and group V monolayers, including the oxides of arsenene and antimonene,^{19,20} hydrogenated and halogenated germanene,^{21} stanene,^{22} and bismuthene,^{23} with sizable bulk gap up to 1.08 eV that is sufficiently large for practical applications at room temperature. The halogenated bismuthene also exhibit diverse topological phases, such as quantum valley Hall insulators^{24} and timereversalinvariant topological superconductors.^{25} So far, experimental observations of QSH effects are reported for HgTe/CdTe and InAs/GaSb quantum wells,^{26,27} and Bi(111) bilayer on substrates.^{28} The exciting properties of these socalled QSH insulators or topological insulators (TI) are triggering extensive research in exploring new candidate TIs for 2D electronics, thermoelectrics,^{29} spintronics, valleytronics, and quantum computation.
Despite the excellent properties of 2D groupIII monochalcogenides themselves, only limited attentions have been paid to their chemical modifications so far. Balakrishnan et al. controllably oxidized the surface of InSe nanolayers by photoannealing and thermalannealing in air, and obtained InSe/In_{2}O_{3} heterostructures as p–n junctions with tunable band gap.^{30} Beechem et al. and Del PozoZamudio et al. showed that oxidation of ultrathin GaSe and InSe films lead to the reduction of photoluminescence.^{31,32} However, the structures, physical, and chemical properties of the modified MX sheets are still unclear and await explorations.
Herein we investigate the electronic and topological properties of oxygen functionalized groupIII monochalcogenides monolayers including GaS, GaSe, GaTe, InS, InSe, and InTe. Firstprinciples calculations reveal that monolayer MX with one side or both sides fully covered by O atoms are energetically and dynamically stable. The chemical modification narrows or even closes the band gap, increases the work function, and reduces the carrier effective masses. The doubleside oxygen functionalized InS, InSe, and InTe sheets are TIs with large bulk gap up to 0.20 eV opened by spin–orbit coupling (SOC), and the lowenergy bands are associated with the s, p_{ x }, and p_{ y } atomic orbitals. These modified MX sheets provide new platforms for exploring novel topological states toward the development of highspeed and dissipationless transport devices.
Results and discussion
In monolayer MX, each chalcogen atom is sp^{3} hybridized with three of the sp^{3} orbitals forming M−X bonds. The remaining orbital is occupied by lonepair electrons and forms a dative bond with an O atom. To functionalize the MX sheets, we consider O atoms chemisorbed on top of the chalcogen sites of GaS, GaSe, GaTe, InS, InSe, and InTe monolayers, fully covering one side or both sides of the 2D sheet as displayed by Fig. 1a. After structural optimization, the O−X bonds are perpendicular to the MX sheets to minimize Coulomb repulsion. The O−S, O−Se, and O−Te bond lengths are about 1.49, 1.66, and 1.83 Å with bond overlap population of 0.47, 0.58, and 0.60, respectively, indicating covalent bonding between O and the underneath chalcogen atoms. The lonepair electrons are captured by the more electronegative O atoms—each O atom gains 0.68–0.77e according to Mulliken charge analysis. Due to the oxygen functionalization, the inplane lattice parameters of the MX sheets expand by 4.14–7.61% and the layer thicknesses (X–X distance) shrink by 0–4.6%, respectively (Table 1 and Table S1 of Supplementary Information). All the modified MX sheets (hereafter denoted as MXO_{0.5} and MXO) present phonon dispersions without imaginary bands, signifying their dynamic stability (Fig. 1d, Fig. S1 and S2 of Supplementary Information). In particular, the oxygen functionalization induces a phonon band at frequency of 800–1100 cm^{−1} corresponding to the outofplane vibration of the O atoms, while all of the pristine monolayers have phonon bands below 400 cm^{−1}.^{12}
To characterize the energetic stability of MXO_{0.5} and MXO, we define the binding energy ∆H as
where E(MXO_{ n }) (n = 0.5 or 1) and E(MX) are the energies of the MXO_{0.5} (or MXO) and MX monolayers, respectively; E(O) is the energy of an isolated O atom. In presence of atomic O, formation of MXO_{0.5} and MXO is energetically favorable with ∆H = −3.11 to −2.17 eV per O atom (Table 1) and kinetically readily. As the O coverage increases, the formation energy raises slightly with energy gain less than 0.3 eV per O atom between the dilute and full coverage (Fig. S34 of Supplementary Information). Therefore, these functionalized MX sheets could be synthesized by the oxygen plasma technique.^{33,34} Although these oxide layers are thermodynamically less stable compared to MX sheets in O_{2} environment, desorption of the O functionalities to form O_{2} molecules involves large kinetic barriers of 1.75–3.23 eV (Fig. S5 of Supplementary Information). Furthermore, ab initio molecular dynamic (AIMD) simulations demonstrate that the MXO_{0.5} and MXO sheets are thermally stable at 300 K (Fig. S67 of Supplementary Information). Thus, these functionalized MX monolayers can stably exist at ambient condition for practical applications.
The simulated Raman spectra of the pristine and functionalized MX monolayers are displayed by Fig. 1c and Fig. S8 of Supplementary Information. Taking monolayer InSe as a representative, the pristine system shows two characteristic peaks at frequencies of 110 and 225 cm^{−1}, both corresponding to the outofplane A_{1} vibration mode. A shoulder peak in the intermediate frequencies around 178 cm^{−1} is attributed to the inplane E mode, consistent with the experimental observations.^{35,36} Upon oxidation, the inplane vibration involving O atoms dominates the active Raman modes, giving rise to a characteristic peak at 197 cm^{−1} for MXO_{0.5} and 180 cm^{−1} for MXO. The outofplane vibration of O atoms induces an additional peak at higher frequency of 867 cm^{−1} and the intensity is stronger for InSeO than for InSeO_{0.5} monolayer, which is distinguishable from pristine InSe sheet and is a signature of the presence of O−Se bonds. The other MX sheets and their functionalized systems exhibit similar features in the Raman spectra as those of InSe, InSeO_{0.5}, and InSeO sheets. Generally, the characteristic peaks undergo red shifts as M and X atoms become heavier.
The oxygen functionalization dramatically affects the electronic band structures of the MX sheets, as demonstrated by Table 1, Fig. 2, and Fig. S9–13 of Supplementary Information. Pristine MX monolayers are semiconductors with indirect band gap of 2.01–3.47 eV calculated by the hybrid HSE06 functional, in good agreement with the experimental values and the previous theoretical reports by the same functional.^{6,37} The PBE functional underestimates the band gap by 0.56–1.02 eV compared to those by the HSE06 functional. The valence band maximum (VBM) is sombreroshape giving effective masses of 1.03–2.09m_{0} (m_{0} is the electron rest mass) for hole carriers. The conduction band minimum (CBM) is parabolic having smaller electron effective masses of 0.15–1.76m_{0}. By singleside oxygen functionalization, the MX monolayers become directgap semiconductors with reduced gap of 0.37–1.51 eV at the Γ point. The VBM and CBM are both parabolic with enhanced dispersion—the effective masses decrease to 0.84–1.35m_{0} for holes and 0.12–1.21m_{0} for electrons, respectively. Upon doubleside functionalization, the band gap is further narrowed to 0.98, 0.12, and 0.08 eV for GaSO, GaSeO, and GaTeO sheets, respectively; meanwhile the InSO, InSeO, and InTeO monolayers become semimetals with the VBM and CBM degenerated at the Γ point. For all the MXO sheets, the CBM is very sharp yielding small electron effective masses of 0.03–0.13m_{0}; the hole effective masses are reduced as well to 1.12–1.66m_{0}. Thus, these modified MX sheets hold high carrier mobilities with sizable direct gap, which are promising for highspeed electronics and optoelectronics. Moreover, the chemisorption of O atoms greatly enhances the polarity of the MX surface. As a consequence, the work function increases to 6.66–7.14 eV for MXO_{0.5} and 8.52–8.99 eV for MXO, respectively, compared to 5.55–6.82 eV for the pristine systems.
Oxygen functionalization of MX monolayers provides the opportunities for modulating the band gap and work function in a wide range and simultaneously enhancing the carrier mobility. To unveil the origin of these peculiar electronic properties, we examine the band projection and partial charge densities of the functionalized MX sheets, as revealed by Fig. 3 and Fig. S14 of Supplementary Information. Pristine MX monolayers have the top valence band (VB) originated from the p_{ z } orbitals of M and X atoms, and the bottom conduction band (CB) dominated by the s orbitals of both types of atoms. Accordingly, the top VB charge densities exhibit the dumbbell p_{ z } orbital character, while the bottom CB charge densities are accumulated in between the M and X atoms showing the inplane σ bond character. In contrast, the MXO_{0.5} and MXO monolayers have the top VB and bottom CB both dominated by the p_{ x } and p_{ y } orbitals of O, M, and X atoms; the s orbitals of M and X atoms also contribute to the bottom CB. The p_{ z } orbitals of all the atoms are hybridized and embedded in the deeper energy levels below −1.5 eV (or above 1.5 eV). The σcharacter band edges may be broader than πcharacter bands giving rise to larger overlap integral and thus responsible for the stronger dispersion and smaller carrier effective masses. The partial charge densities of the frontier bands are localized individually on the O and X atoms, indicating the occupancy of antibonding states between O and X atoms that leads to narrowing of band gap. The σcharacter band edges would be beneficial for manipulating the band gap by inplane strains.^{18}
Intuitively, the functionalized MX monolayers with large atomic numbers may have prominent SOC effect. As demonstrated by Fig. 2, Fig. S1213 of Supplementary Information, the SOC effect indeed opens indirect gap of 0.08, 0.13, and 0.21 eV for the InSO, InSeO, and InTeO monolayers, respectively, with VBM shifted slightly away from the Γ point. For the other semiconducting systems, the electronic band structures are almost identical to those without including SOC. The SOCinduced transition from semimetal to insulator in the InXO monolayers suggests that they are potential 2D TI.^{38}
To explore the topological properties of the InSO, InSeO, and InTeO monolayers, we firstly calculate the Z_{2} topological invariant by two methods, i.e. the Wannier center of charges (WCCs) method^{39} and the lattice method.^{40} Z_{2} = 1 characterizes a nontrivial band topology, while Z_{2} = 0 corresponds to a trivial insulator. As plotted in Fig. 4, by counting the number of crossings of any arbitrary horizontal reference line, the WCCs curves cross any reference lines odd times, giving Z_{2} = 1 for the InSO, InSeO, and InTeO monolayers, which are also confirmed by the lattice method. In other words, they are all TIs with appreciable bulk gap up to 0.21 eV. Hence, it is possible to observe QSH effects in the InXO monolayers at room temperature.
In addition to the Z_{2} topological invariant, the helical gapless edge modes inside the bulk energy gap provide a more intuitive picture to vindicate the nontrivial topological properties of the InXO monolayers. Using an iterative method to obtain the surface Green’s function of the semiinfinite system,^{41} one can calculate the dispersion of the edge states.^{42} As shown by Fig. 4, odd number (one) pairs of helical edge states traverse the bulk band gap. These kinds of edge states are protected from backscattering by the timereversal symmetry, enabling dissipationless transport in these functionalized sheets.^{43}
In order to understand the topological properties, we build the k · p effective model. As revealed by Fig. 2, the band is almost twofold degenerate with negligible splitting near the Fermi level. Thus, we can consider the InXO (X = S, Se, Te) sheet centrosymmetric. The same strategy is used to derive to the BHZ model on HgTe quantum well^{26} and argue the nontrivial topological properties of strained HgTe,^{44} which is also noncentrosymmetric essentially. In addition, the InXO monolayer has mirror reflection symmetry M_{ z } = is_{ z } and time reversal symmetry T = iKs_{ z } (K is the complex conjugation). Given the three symmetries, to the lowest order the k · p Hamiltonians near Γ may be written as
where λ is the effective SOC strength and ∆ indicates a mass term without SOC (the system is topological nontrivial when λ > ∆ and is trivial when λ < ∆); Pauli matrix s and σ act on the spin and orbital space, respectively. The parameters C, A, B > 0 can be determined by fitting the band structure from density functional theory (DFT) calculation. For the typical InSeO monolayer, one has A = 1.85 eV Å, B = 8.50 eV Å^{2}, C = 9.21 eV Å^{2}, ∆ = 0 and λ = 0.067 eV. In the InXO sheet, inversion symmetry is softly broken, and inversion symmetry broken terms will be present. Nevertheless, since such terms are small and do not lead to any level crossings at the Fermi energy, one can first analyze the physics in the absence of these terms and then argue by the principle of adiabatic continuity that the same topological physics remains valid when the inversion breaking terms are taken into account.
Furthermore, the bulk gap of InXO monolayers is sensitive to inplane strains due to the σcharacter band edges. As displayed by Fig. 5 and Fig. S15 of Supplementary Information, the gap can be rigidly enlarged under tensile strains within 6%, up to 0.10, 0.15, and 0.24 eV for InSO, InSeO, and InTeO monolayers, respectively. The bulk gap sustains under compressive strains within 6%, and is reduced down to 0.07, 0.10, and 0.17 eV for InSO, InSeO, and InTeO monolayers, respectively. In all situations, the band dispersions are not severely disrupted. It is worth noting that the SOC gap never closes during the whole strain range; thus all the strained systems share the same nontrivial topology as the unstrained ones. In short, the bulk gap of InXO monolayers can be effectively modulated by external strains, and their TI phases are robust under moderate compressive/tensile strains (≤6%).
In summary, we propose to tailor the electronic and topological properties of groupIII monochalcogenides monolayers (MX with M = Ga, In; X = S, Se, Te) by oxygen functionalization. Our firstprinciples calculations demonstrate that these modified MX sheets possess appreciable energetic, thermal, and chemical stabilities. The oxygen functionalization effectively tailor the electronic structure by narrowing or even closing the band gap, reducing the carrier effective masses, and increasing the work function. Most excitingly, monolayer InS, InSe and InTe with doubleside oxygen functionalization are 2D TI; their lowenergy bands are dominated by the hybridized p_{ x } and p_{ y } orbitals of O, In, and S (Se, Te) atoms, giving rise to large bulk gap up to 0.21 eV. These functionalized MX sheets, naturally against further surface oxidation and degradation, provide an ideal platform for realizing QSH effect at room temperature, toward the development high speed and dissipationless transport devices.
Methods
DFT calculations were performed by the Vienna ab initio simulation package (VASP) using the planewave basis with energy cutoff of 450 eV and the projector augmented wave potentials.^{45} Within the generalized gradient approximation, the PBE exchangecorrelation functional was used for the structure, energy, phonon dispersion, and Raman spectrum calculations,^{46} and the hybrid HSE06 functional was adopted for the electronic band structure calculations.^{47} We used the primitive unit cell of monolayer MX with a vacuum region of 16 Å in the vertical direction to avoid interactions between the layers. The Brillouin zone was sampled by 16 × 16 × 1 uniform k point mesh. The 2D structures were fully optimized for the electronic and cell degrees of freedom with threshold of 10^{6} eV for the total energy and 10^{−3} eV/Å for the forces on each atom. Based on the equilibrium structures, the phonon dispersions were then calculated by density functional perturbation theory as implemented in the Phonopy package.^{48} The Raman spectrum and bond population were computed by CASTEP using the planewave basis with energy cutoff of 1000 eV and normconserving pseudopotentials.^{49}
In order to assess the thermal stability of the MXO_{0.5} and MXO monolayers, AIMD simulations were performed within the NVT ensemble at temperature of 300 K and time step of 1.0 fs for a total of 20 ps. The kinetic stability of these functionalized MX sheets were examined by the climbingimage nudged elastic band method implemented in VASP. A supercell consisting of 4 × 4 unit cells of MX monolayer was adopted for oxygen desorption and O_{2} formation. Seven images were used to mimic the reaction path. The intermediate images were relaxed until the perpendicular forces were smaller than 0.02 eV/Å.
By using WANNIER90 code, the maximally localized Wannier functions were constructed, and the Berry curvature was obtained.^{50} Based on the constructed Wannier functions, we directly calculated the Z_{2} topological invariant by both WCCs method^{39} and the lattice method,^{40} and used an iterative method^{41} to obtain the surface Green’s function of the semiinfinite system from which one can stimulate the dispersion of the edge states.
Data availability
The data that support the findings of this study are available from the corresponding authors upon reasonable request.
References
 1.
Lieth, R. Preparation and Crystal Growth of Materials with Layered Structures (Springer Press, Dordrecht, 1977).
 2.
Xu, K. et al. Synthesis, properties and applications of 2D layered M^{III}X^{VI} (M= Ga, In; X= S, Se, Te) materials. Nanoscale 8, 16802–16818 (2016).
 3.
Hu, P. et al. Highly responsive ultrathin GaS nanosheet photodetectors on rigid and flexible substrates. Nano Lett. 13, 1649–1654 (2013).
 4.
Lei, S. et al. Synthesis and photoresponse of large GaSe atomic layers. Nano Lett. 13, 2777–2781 (2013).
 5.
Lei, S. et al. An atomically layered InSe avalanche photodetector. Nano Lett. 15, 3048–3055 (2015).
 6.
Zhuang, H. L. & Hennig, R. G. Singlelayer groupIII monochalcogenide photocatalysts for water splitting. Chem. Mater. 25, 3232–3238 (2013).
 7.
Late, D. J. et al. GaS and GaSe ultrathin layer transistors. Adv. Mater. 24, 3549–3554 (2012).
 8.
Bandurin, D. A. et al. High electron mobility, quantum Hall effect and anomalous optical response in atomically thin InSe. Nat. Nanotechnol. 12, 223–227 (2017).
 9.
Sucharitakul, S. et al. Intrinsic electron mobility exceeding 10^{3} cm^{2}/(V·s) in multilayer InSe FETs. Nano Lett. 15, 3815–3819 (2015).
 10.
Liu, F. et al. Highsensitivity photodetectors based on multilayer GaTe flakes. ACS Nano 8, 752–760 (2014).
 11.
Tamalampudi, S. R. et al. High performance and bendable fewlayered InSe photodetectors with broad spectral response. Nano Lett. 14, 2800–2806 (2014).
 12.
Guo, Y., Zhou, S., Bai, Y. & Zhao, J. Enhanced piezoelectric effect in Janus groupIII chalcogenide monolayers. Appl. Phys. Lett. 110, 163102 (2017).
 13.
Han, G., Chen, Z. G., Drennan, J. & Zou, J. Indium selenides: structural characteristics, synthesis and their thermoelectric performances. Small 10, 2747–2765 (2014).
 14.
Harvey, A. et al. Preparation of gallium sulfide nanosheets by liquid exfoliation and their application as hydrogen evolution catalysts. Chem. Mater. 27, 3483–3493 (2015).
 15.
Qiu, J. et al. Ordered and reversible hydrogenation of silicene. Phys. Rev. Lett. 114, 126101 (2015).
 16.
Eda, G., Fanchini, G. & Chhowalla, M. Largearea ultrathin films of reduced graphene oxide as a transparent and flexible electronic material. Nat. Nanotechnol. 3, 270–274 (2008).
 17.
Zhu, L. et al. Blue phosphorene oxide: straintunable quantum phase transitions and novel 2D emergent fermions. Nano Lett. 16, 6548–6554 (2016).
 18.
Li, Y. & Chen, X. Dirac fermions in bluephosphorus. 2D Mater. 1, 031002 (2014).
 19.
Wang, Y. P. et al. Twodimensional arsenene oxide: a realistic largegap quantum spin Hall insulator. Appl. Phys. Lett. 110, 213101 (2017).
 20.
Zhang, S. et al. Antimonene oxides: emerging tunable direct bandgap semiconductor and novel topological insulator. Nano Lett. 17, 3434–3440 (2017).
 21.
Si, C. et al. Functionalized germanene as a prototype of largegap twodimensional topological insulators. Phys. Rev. B 89, 115429 (2014).
 22.
Xu, Y. et al. Largegap quantum spin Hall insulators in tin films. Phys. Rev. Lett. 111, 136804 (2013).
 23.
Liu, C.C. et al. Lowenergy effective Hamiltonian for giantgap quantum spin Hall insulators in honeycomb Xhydride/halide (X= N–Bi) monolayers. Phys. Rev. B 90, 085431 (2014).
 24.
Song, Z. et al. Quantum spin Hall insulators and quantum valley Hall insulators of BiX/SbX (X= H, F, Cl and Br) monolayers with a record bulk band gap. NPG Asia Mater. 6, e147 (2014).
 25.
Yang, F., Liu, C.C., Zhang, Y.Z., Yao, Y. & Lee, D.H. Timereversalinvariant topological superconductivity in ndoped BiH. Phys. Rev. B 91, 134514 (2015).
 26.
Bernevig, B. A., Hughes, T. L. & Zhang, S.C. Quantum spin Hall effect and topological phase transition in HgTe quantum wells. Science 314, 1757–1761 (2006).
 27.
Knez, I., Du, R.R. & Sullivan, G. Evidence for helical edge modes in inverted InAs/GaSb quantum wells. Phys. Rev. Lett. 107, 136603 (2011).
 28.
Yang, F. et al. Spatial and energy distribution of topological edge states in single Bi(111) bilayer. Phys. Rev. Lett. 109, 016801 (2012).
 29.
Xu, N., Xu, Y. & Zhu, J. Topological insulators for thermoelectrics. npj Quantum Mater. 2, 51 (2017).
 30.
Balakrishnan, N. et al. Engineering p–n junctions and bandgap tuning of InSe nanolayers by controlled oxidation. 2D Mater. 4, 025043 (2017).
 31.
Del PozoZamudio, O. et al. Photoluminescence of twodimensional GaTe and GaSe films. 2D Mater. 2, 035010 (2015).
 32.
Beechem, T. E. et al. Oxidation of ultrathin GaSe. Appl. Phys. Lett. 107, 173103 (2015).
 33.
Hossain, M. Z. et al. Chemically homogeneous and thermally reversible oxidation of epitaxial graphene. Nat. Chem. 4, 305–309 (2012).
 34.
Zhou, S., Sherpa, S. D., Hess, D. W. & Bongiorno, A. Chemical bonding of partially fluorinated graphene. J. Phys. Chem. C 118, 26402–26408 (2014).
 35.
Lei, S. et al. Surface functionalization of twodimensional metal chalcogenides by Lewis acid–base chemistry. Nat. Nanotechnol. 11, 465–471 (2016).
 36.
Yang, Z. et al. Waferscale synthesis of highquality semiconducting twodimensional layered InSe with broadband photoresponse. ACS Nano 11, 4225–4236 (2017).
 37.
Jung, C. S. et al. Redtoultraviolet emission tuning of twodimensional gallium sulfide/selenide. ACS Nano 9, 9585–9593 (2015).
 38.
Kane, C. L. & Mele, E. J. Quantum spin Hall effect in graphene. Phys. Rev. Lett. 95, 226801 (2005).
 39.
Gresch, D. et al. Z2Pack: Numerical implementation of hybrid Wannier centers for identifying topological materials. Phys. Rev. B 95, 075146 (2017).
 40.
Fukui, T. & Hatsugai, Y. Quantum spin Hall effect in three dimensional materials: Lattice computation of Z2 topological invariants and its application to Bi and Sb. J. Phys. Soc. Jpn. 76, 053702 (2007).
 41.
Sancho, M. L., Sancho, J. L., Sancho, J. L. & Rubio, J. Highly convergent schemes for the calculation of bulk and surface Green functions. J. Phys. F 15, 851–858 (1985).
 42.
Wu, Q., Zhang, S., Song, H.F., Troyer, M. & Soluyanov, A. A. WannierTools: an opensource software package for novel topological materials. Preprint at arXiv:1703.07789 (2017).
 43.
Qi, X.L. & Zhang, S.C. Topological insulators and superconductors. Rev. Mod. Phys. 83, 1057–1110 (2011).
 44.
Fu, L. & Kane, C. L. Topological insulators with inversion symmetry. Phys. Rev. B 76, 045302 (2007).
 45.
Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector augmentedwave method. Phys. Rev. B 59, 1758 (1999).
 46.
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
 47.
Heyd, J., Scuseria, G. E. & Ernzerhof, M. Hybrid functionals based on a screened Coulomb potential. J. Chem. Phys. 118, 8207–8215 (2003).
 48.
Togo, A., Oba, F. & Tanaka, I. Firstprinciples calculations of the ferroelastic transition between rutiletype and CaCl_{2}type SiO_{2} at high pressures. Phys. Rev. B 78, 134106 (2008).
 49.
Clark, S. J. et al. First principles methods using CASTEP. Z. Krist.Cryst. Mater. 220, 567–570 (2005).
 50.
Mostofi, A. A. et al. Wannier90: a tool for obtaining maximallylocalised Wannier functions. Comput. Phys. Commun. 178, 685–699 (2008).
Acknowledgements
This work was supported by the National Natural Science Foundation of China (11504041, 11574040, 11774028, 11574029, and 11734003), the National Key R&D Program of China (No. 2016YFA0300600), the MOST Project of China (No. 2014CB920903), the China Postdoctoral Science Foundation (2015M570243 and 2016T90216), the Fundamental Research Funds for the Central Universities of China (DUT16LAB01 and DUT17LAB19), Basic Research Funds of Beijing Institute of Technology (2017CX01018), and the Supercomputing Center of Dalian University of Technology.
Author information
Affiliations
Contributions
S.Z. conceived the idea, performed the DFT calculations and wrote the manuscript. C.C.L. performed the calculations of topological properties. J.Z. and Y.Y. guided the research. All authors contributed to the discussion and data interpretation and have read and approved the final manuscript.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Zhou, S., Liu, CC., Zhao, J. et al. Monolayer groupIII monochalcogenides by oxygen functionalization: a promising class of twodimensional topological insulators. npj Quant Mater 3, 16 (2018). https://doi.org/10.1038/s4153501800890
Received:
Revised:
Accepted:
Published:
Further reading

Coexistence of intrinsic piezoelectricity and nontrivial band topology in monolayer InXO (X = Se and Te)
Journal of Materials Chemistry C (2021)

Influence of different exchange–correlation potentials on twisted structures of bilayer XS2 (X = Mo, Cr)
Computational Materials Science (2021)

Computational identification of efficient 2D Aluminium chalcogenides monolayers for optoelectronics and photocatalysts applications
Applied Surface Science (2021)

Drastic reduction of thermal conductivity in hexagonal AX (A = Ga, In & Tl, X = S, Se & Te) monolayers due to alternative atomic configuration
Nano Energy (2021)

Surface Functionalization Tailored Electronic Structure and Magnetic Properties of TwoDimensional CrC2 Monolayers
The Journal of Physical Chemistry C (2020)